# Introduction to Materials Science and Engineering

60

## Full text

(1)

### Eun Soo Park

Office: 33‐313

Telephone: 880‐7221 Email: espark@snu.ac.kr

Office hours: by appointment

2019 Fall

09. 19. 2019

(2)

### Fundamentals of Crystallography

I. Crystal Structures

- Lattice, Unit Cells, Crystal system

II. Crystallographic Points, Directions, and Planes

- Point coordinates, Crystallographic directions, Crystallographic planes

III. Crystalline and Noncrystalline Materials

- Single crystals, Polycrystalline materials, Anisotropy, Noncrystalline solids

(3)

### Stacking of atoms in solid

Finding stable position

(4)

### Lattice

– 3D point array in space, such that each point has

identical surroundings. These points may or may not coincide with atom positions.

– Simplest case : each atom its center of gravity

point or space lattice pure mathematical concept example: sodium (Na) ; body centered cubic

: 결정 공간상에서 점들의 규칙적인 기하학적 배열

(5)

### 14 Bravais Lattice -

Only 14 different types of unit cells

are required to describe all lattices using symmetry

cubic hexagonal rhombohedral (trigonal) tetragonal orthorhombic monoclinic triclinic

P I F C 5

(6)

– ex) P: q,r,s

### cubic unit cell

Chapter 3.5 Point coordinates

(7)

(8)

### Lattice plane (Miller indices)

m00, 0n0, 00p: define lattice plane m, n, ∞ : no intercepts with axes

z

### p

Miller indicies ; defined as the smallest integral multiples of the reciprocals of the plane

intercepts on the axes Plane (hkl) Family of planes {hkl} Intercepts @ (mnp) 2 1 3 Reciprocals ½ 1 1/3 Miller indicies 3 6 2 (362) plane (362)

(9)

### in Hexagonal system

w w u v t v v v u t u u          ' 2 ' 2 ' ' ) ' ' 2 ( 3 1 ) ' ' 2 ( 3 1 w w u v v v u u      Miller to Miller-Bravais 3axis to 4 axis system Miller-Bravais to Miller 4 to 3 axis

1

2

1

2

3

### 

Directions

Conversion of 4 index system (Miller-Bravais) to 3 index (Miller)

Ex. M [100] u=(1/3)(2*1-0)=2/3 v=(1/3)(2*0-1)=-1/3 w=0 => 1/3[2 -1 -1 0] Ex. M-B [1 0 -1 0] u’=2*1+0=2 v’=2*0+1=1 w’=0 => [2 1 0] 9

(10)

### Fundamentals of Crystallography

III. Crystalline ↔ Noncrystalline Materials

- Single crystals, Polycrystalline materials, Anisotropy - Quasicrystals

- Noncrystalline solids : Amorphous solid

Contents for today’s class

(11)

### Some

engineering applications require single crystals:

• Crystal properties reveal features of atomic structure.

(Courtesy P.M. Anderson)

--Ex: Certain crystal planes in quartz fracture more easily than others. --diamond single crystals

Natural and artificial

Fig. 8.30(c), Callister 6e. (Fig. 8.30(c) courtesy of Pratt and Whitney).

(Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.)

### AS BUILDING BLOCKS

III. Crystalline ↔ Noncrystalline Materials

(12)

4 Fold Anisotropic Surface Energy/2 Fold Kinetics, Many Seeds

: Liquid Solid

(13)

### Grain Boundaries

(14)

• Single Crystals

-Properties vary with direction: anisotropic.

-Example: the modulus

of elasticity (E) in BCC iron:

• Polycrystals

-Properties may/may not vary with direction.

-If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa)

-If grains are textured, anisotropic.

200 m

Data from Table 3.3,

Callister 7e.

(Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd

ed., John Wiley and Sons, 1989.)

Callister 7e.

(Fig. 4.14(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].)

### Single vs Polycrystals

E (diagonal) = 273 GPa

(15)

Most engineering materials are polycrystals.

• Nb-Hf-W plate with an electron beam weld. • Each "grain" is a single crystal.

• If grains are randomly oriented,

overall component properties are not directional.

• Grain sizes typ. range from 1 nm to 2 cm

(i.e., from a few to millions of atomic layers).

Adapted from Fig. K, color inset pages of Callister 5e.

(Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany)

1 mm

### Polycrystals

Isotropic Anisotropic

(16)

### Polymorphism

• Two or more distinct crystal structures for the same material (allotropy/polymorphism)

titanium, -Ti carbon diamond, graphite BCC FCC BCC 1538ºC 1394ºC 912ºC -Fe -Fe -Fe liquid iron system

(17)

• Demonstrates "polymorphism" The same atoms can have more than one

crystal structure.

### AN IRON WIRE

Temperature, C BCC Stable FCC Stable 914 1391 1536 shorter longer! shorter! longer

Tc 768 magnet falls off

BCC Stable Liquid

heat up

cool down

(18)

### Non-crystalline Materials

Amorphous materials

a wide diversity of materials can be rendered amorphous

indeed almost all materials can. - metal, ceramic, polymer

ex) amorphous metallic alloy (1960) - glassy/non-crystalline material

cf) amorphous vs glass

- random atomic structure (short range order) - showing glass transition.

- retain liquid structure

- rapid solidification from liquid state

Amorphous

(19)

Obsidian is a naturally occurring volcanic glass formed as an extrusive igneous rock. It is produced when felsic lava extruded from a volcano cools rapidly with minimum crystal growth. Obsidian is commonly found within the margins of rhyolitic lava flows known as obsidian flows, where the chemical composition (high silica content) induces a high viscosity and polymerization degree of the lava. The inhibition of atomic diffusion through this highly viscous and polymerized lava explains the lack of

crystal growth. Because of this lack of crystal structure, abcde obsidian blade edges can reach almost molecular thinness,

leading to its ancient use as projectile points and blades, and its modern use as surgical scalpel blades.

(20)

### Glass formation: stabilizing the liquid phase

W. Klement, R.H. Willens, P. Duwez, Nature 1960; 187: 869.

2 . 0 *    mix m T m T mix m T T

in most of glass forming alloys

by I.W. Donald et al, J. Non-Cryst. Solids, 1978;30:77. - Relative decrease of melting temperature (where, , = mole fraction, = melting point)   i m i mix m xT T i x i m T Au Si 0 10 20 30 40 50 60 70 80 90 100 100 300 500 700 900 1100 1300 1500 18.6 363 1064.4 1414 Liquid deep eutectic ΔT* = 0.679

Rapid splat quenching

liquid metal droplet

laser trigger metal piston metal anvil t = 20 μm l = 3 cm w = 2 cm Tmmix Tm

First metallic glass (Au80Si20) produced by splat quenching at Caltech by Pol Duwez in 1957.

(21)

### Bulk glass formation in the Pd-/Ni-/Cu-/Zr- system

(22)
(23)

:Metallic Glasses OfferaUnique Combination ofHigh Strength and High Elastic Limit Metallic glass Polymers Woods Silica Titanium alloys Steels 2500 2000 1500 1000 500 0 Elastic Limit (%) 0 1 2 3

Strength vs. Elastic Limit for Several Classes of Materials

(24)

Superior thermo‐plastic formability

:possibleto fabricatecomplexstructurewithoutjoints

Seamaster Planet Ocean Liquidmetal® Limited Edition

Ideal for small expensive IT equipment manufacturing Multistep processing can be solved by simple casting

Processing metals as efficiently as plastics: net‐shape forming! Processing metals as efficiently as plastics: net‐shape forming!

(25)

## What are Quasicrystals?

(26)

### … only certain symmetries are possible

A tessellation or tiling of the plane is

(27)

According to the well-known theorems of crystallography, only certain symmetries are allowed: the symmetry of a square, rectangle, parallelogram, triangle or hexagon, but not others, such as pentagons.

Symmetry axes compatible

with periodicity

(28)

### Crystals can only exhibit certain symmetries

Crystals can only exhibit these same rotational symmetries* ..and the symmetries determine

many of their physical properties and applications * In 3D, there can be different rotational symmetries

along different axes, but they are restricted to the same set (2-, 3-, 4-, and 6-fold)

(29)

### were first discovered in the laboratory by

Daniel Shechtman, Ilan Blech, Denis Gratias and John Cahn

### in a beautiful study of an alloy of Al and Mn

(30)

D. Shechtman, I. Blech, D. Gratias, J.W. Cahn (1984)

6

### Mn

(31)

Their surprising claim:

6

(32)

### of repeating units

D. Levine and P.J. Steinhardt (1984)

### Similar to crystals, BUT…

(33)

LEFT: Fig. 1 (A) The original khatyrkite-bearing sample used in the study. The lighter-colored material on the exterior contains a mixture of spinel, augite, and olivine. The dark material consists predominantly of khatyrkite (CuAl2) and cupalite (CuAl) but also

includes granules, like the one in (B), with composition Al63Cu24Fe13. The diffraction patterns in Fig. 4 were obtained from the thin

region of this granule indicated by the red dashed circle, an area 0.1 μm across. (C) The inverted Fourier transform of the HRTEM image taken from a subregion about 15 nm across displays a homogeneous, quasiperiodically ordered, fivefold symmetric, real space pattern characteristic of quasicrystals.

RIGHT: Diffraction patterns obtained from natural quasicrystal grain

### Discovery of a Natural Quasicrystal

L Bindi, P. Steinhardt, N. Yao and P. Lu

Science 324, 1306 (2009)

(34)

### Quasicrystal

A new ordered phase showing the apparent fivefold symmetry was observed by Sastry et al. [Mater. Res.

Bull. 13: 1065-1070] in 1978 in a rapidly solidified Al-Pd alloy, but was interpreted to arise from a microstructure Consisting of a series of fine twins. This was later shown to be a two-dimensional (or decagonal) qasicrystal.

(35)

### Quasicrystals

: materials whose structure cannot be understood within classical crystallography rules.

“Quasiperiodic lattices”, with long-range order but without periodic translations in three dimensions

### • sharp diffraction patterns

http://www.youtube.com/watch?v=k_VSpBI5EGM Crystal with 5 fold symmetry Mathematically impossible but exist

1984 Al86Mn14 alloy : rapidly solidified ribbon_Shectman et al.

(36)

### Atomic arrangement in the solid state

 Solid materials are classified according to the regularity with

which atoms and ions are arranged with respect to one another.

 So, how are they arranged ?

(a) periodically – having long range order in 3-D (b) quasi-periodically

(c) randomly – having short range order with the characteristics of bonding type but losing the long range order

Crystal

Amorphous Quasicrystal

(37)

• tend to be densely packed.

• have several reasons for dense packing:

- Typically, only one element is present, so all atomic radii are the same.

- Metallic bonding is not directional.

- Nearest neighbor distances tend to be small in order to lower bond energy.

• have the simplest crystal structures.

We will look at three such structures...

### The Structure of Crystalline Solids

(38)

• Rare due to poor packing (only 84Polonium has this structure)

• Close-packed directions are cube edges.

• Coordination # = 6 (# nearest neighbors)

(Courtesy P.M. Anderson)

(39)

### * Coordination Number

In chemistry and crystallography, the coordination number (CN) of a central atom in a molecule or crystal is the number of its nearest neighbor.

In chemistry the emphasis is on bonding structures in molecules or ions and the CN of an atom is determined by simply counting the other of atoms to which it is bonded (by either single or multiple bonds).

The solid-state structure of crystals often have less clearly defined bonds, so a simpler model is used, in which the atoms are represented by touching spheres. In this model the CN of an atom is the number of other atoms which it touches. For an atom in the interior of a crystal lattice, the number of atoms touching the given atom is the bulk coordination number, for an atom at a surface of a crystal this is the surface coordination number.

(40)
(41)

### Coordination Number

(42)

APF = Volume of atoms in unit cell* Volume of unit cell

*assume hard spheres

• APF for a simple cubic structure = 0.52

APF = a3 4 3 (0.5a)3 1 atoms

unit cell atom

volume unit cell volume close-packed directions a R=0.5a contains 8 x 1/8 = 1 atom/unit cell

Adapted from Fig. 3.19, Callister 6e.

### simple cubic

(43)

• Coordination # = 8

Callister 7e.

(Courtesy P.M. Anderson)

• Atoms touch each other along cube diagonals.

--Note: All atoms are identical; the center atom is shaded differently only for ease of viewing.

### (2) Body Centered Cubic Structure (BCC)

ex: Cr, W, Fe (), Tantalum, Molybdenum

2 atoms/unit cell: 1 center + 8 corners x 1/8

(44)
(45)

### Body Centered Cubic (BCC)

• Close packed directions are cube diagonals <111> • 2 atoms / unit cell (1 + 8 x 1/8) aBCC = 4r/31/2

• Highest density plane {110} Coordination # = 8 • Cr, Fe, W, etc.

BCC

### r

• Coordination # = 8

(46)

a length = 4R = a 2 a 3 a R

• APF for a body-centered cubic structure = 0.68

Close-packed directions: length = 4R

= 3 a

Unit cell contains: 1 + 8 x 1/8

= 2 atoms/unit cell

### ATOMIC PACKING FACTOR: BCC

APF = a3 4 3 ( 3a/4)3 2 atoms

unit cell volumeatom

unit cell volume

Close-packed directions <111>

3 a

Highest density planes {110}

(47)

### {110} Family

(48)
(49)

a length = 4R = a 2 a 3 a R

• APF for a body-centered cubic structure = 0.68

Close-packed directions: length = 4R

= 3 a

Unit cell contains: 1 + 8 x 1/8

= 2 atoms/unit cell

### ATOMIC PACKING FACTOR: BCC

APF = a3 4 3 ( 3a/4)3 2 atoms

unit cell volumeatom

unit cell volume

Close-packed directions <111>

3 a

Highest density planes {110}

(50)

### Planar Density of (100) Iron

At T < 912C iron has the BCC structure.

(100) Radius of iron R = 0.1241 nm R 3 3 4 a

Adapted from Fig. 3.2(c), Callister 7e.

2D repeat unit = Planar Density = a2 1 atoms 2D repeat unit = nm2 atoms 12.1 m2 atoms = 1.2 x 1019 1 2 R 3 3 4 area 2D repeat unit

(51)

### Planar Density of (111) Iron

(111) plane 1 atom in plane/ unit surface cell atoms in plane

atoms above plane atoms below plane

a h 2 3 

### 2

1 = = nm2 atoms 7.0 m2 atoms 0.70 x 1019 3 2 R 3 16 Planar Density = atoms 2D repeat unit area 2D repeat unit 3 3 3 2 2 R 3 16 R 3 4 2 a 3 ah 2 area     51

(52)

(53)

53

(54)

### A

(55)

• Coordination # = 12

Adapted from Fig. 3.1, Callister 7e.

(Courtesy P.M. Anderson)

• Atoms touch each other along face diagonals.

--Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing.

### (3) Face Centered Cubic Structure (FCC)

ex: Al, Cu, Au, Pb, Ni, Pt, Ag

4 atoms/unit cell: 6 face x 1/2 + 8 corners x 1/8

(56)

APF = a3 4 3 ( 2a/4)3 4 atoms

unit cell volumeatom

unit cell volume Unit cell contains: 6 x 1/2 + 8 x 1/8 = 4 atoms/unit cell

a

• APF for a face-centered cubic structure = 0.74

Close-packed directions: length = 4R = 2 a Adapted from Fig. 3.1(a), Callister 6e.

<110> {111}

(57)

### HCP

A-B-A-B-A-….. A-B-C-A-B-C-….. A position B position C position

(58)

• Coordination # = 12

• ABAB... Stacking Sequence

• APF = 0.74

• 3D Projection • 2D Projection

A sites

B sites

A sites Bottom layer

Middle layer

Top layer

Adapted from Fig. 3.3, Callister 6e.

### STRUCTURE (HCP)

<1120> (0001) Close-packed direction : plane :

(59)

### I. Atomic arrangement in the solid state

 Solid materials are classified according to the regularity with

which atoms and ions are arranged with respect to one another.

 So, how are they arranged ?

(a) periodically – having long range order in 3-D (b) quasi-periodically

(c) randomly – having short range order with the characteristics of bonding type but losing the long range order

Crystal

Amorphous Quasicrystal

Crystal: Perfection → Imperfection

59

(60)

Updating...

Updating...